LMucko/crystallography-open-database huggingface dataset:
Neue ternaere Fluoride des Zinks: Sr Zn F4 und Ca Zn F4
von Schnering, H.G.; Bleckmann, P.; Naturwissenschaften 52 (1965) 538–538; doi:

data_1529059
_publ_section_title
;
 Neue ternaere Fluoride des Zinks: Sr Zn F4 und Ca Zn F4
;
_journal_name_full               Naturwissenschaften
_journal_page_first              538
_journal_page_last               538
_journal_volume                  52
_journal_year                    1965
_chemical_formula_sum            'F4 Sr Zn'
_chemical_name_systematic        'Sr Zn F4'
_space_group_IT_number           88
_symmetry_space_group_name_Hall  'I 4bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.448
_cell_length_b                   5.448
_cell_length_c                   11.657
_cell_volume                     345.988
_citation_journal_id_ASTM        NATWAY
_cod_data_source_file            vonSchnering_NATWAY_1965_302.cif
_cod_data_source_block           F4Sr1Zn1
_cod_original_cell_volume        345.9879
_cod_original_sg_symbol_Hall     '-I 4ad (x,y+1/4,z+1/8)'
_cod_original_formula_sum        'F4 Sr1 Zn1'
_cod_database_code               1529059
Neue ternaere Fluoride des Zinks: Sr Zn F4 und Ca Zn F4
von Schnering, H.G.; Bleckmann, P.; Naturwissenschaften 52 (1965) 538–538; doi:

data_1529060
_publ_section_title
;
 Neue ternaere Fluoride des Zinks: Sr Zn F4 und Ca Zn F4
;
_journal_name_full               Naturwissenschaften
_journal_page_first              538
_journal_page_last               538
_journal_volume                  52
_journal_year                    1965
_chemical_formula_sum            'Ca F4 Zn'
_chemical_name_systematic        'Ca Zn F4'
_space_group_IT_number           88
_symmetry_space_group_name_Hall  'I 4bw -1bw'
_symmetry_space_group_name_H-M   'I 41/a :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.323
_cell_length_b                   5.323
_cell_length_c                   11.012
_cell_volume                     312.018
_citation_journal_id_ASTM        NATWAY
_cod_data_source_file            vonSchnering_NATWAY_1965_303.cif
_cod_data_source_block           Ca1F4Zn1
_cod_original_cell_volume        312.0176
_cod_original_sg_symbol_Hall     '-I 4ad (x,y+1/4,z+1/8)'
_cod_original_formula_sum        'Ca1 F4 Zn1'
_cod_database_code               1529060
Single-Crystal Structure and Magnetic Behavior of a Molecule-Based Ferrimagnet Mn[Mn0.2Cr0.8(CN)6]Â·4H2O
Shen Xiaoping; Li Yizhi; Guo Guocong; Xu Zheng; Song You; European Journal of Inorganic Chemistry 2007 (2007) 1698–1702; doi:

data_4031278
_publ_section_title
;
 Single-Crystal Structure and Magnetic Behavior of a Molecule-Based
 Ferrimagnet Mn[Mn0.2Cr0.8(CN)6]&#x00C2;&#x00B7;4H2O
;
_journal_name_full               'European Journal of Inorganic Chemistry'
_journal_page_first              1698
_journal_page_last               1702
_journal_volume                  2007
_journal_year                    2007
_chemical_formula_sum            'C6 H8 Cr0.8 Mn1.2 N6 O4'
_chemical_name_systematic        'Mn (Mn0.2 Cr0.8 (C N)6) (H2 O)4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.7632
_cell_length_b                   10.7632
_cell_length_c                   10.7632
_cell_volume                     1246.879
_citation_journal_id_ASTM        EJICFO
_cod_data_source_file            ShenXiaoping_EJICFO_2007_1313.cif
_cod_data_source_block           C6H8Cr0.8Mn1.2N6O4
_cod_database_code               4031278
Synthesis, Structure, and Magnetic Properties of Precursors to LiMO2 Battery Materials
Tey, S.L.; Reddy, M.V.; Ding, J.; Chowdary, B.V.R.; Rao, G.V.S.; Yi, J.; Vittal, J.J.; Chemistry of Materials (1,1989-) 18 (2006) 1587–1594; doi:

data_4002448
_publ_section_title
;
 Synthesis, Structure, and Magnetic Properties of Precursors to LiMO2
 Battery Materials
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              1587
_journal_page_last               1594
_journal_volume                  18
_journal_year                    2006
_chemical_formula_sum            'C3 H12 Li N6 Ni O7.5'
_chemical_name_systematic        '(Li (H2 O) Ni (N2 H3 C O2)3) (H2 O)0.5'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.262
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.4868
_cell_length_b                   4.9676
_cell_length_c                   11.261
_cell_volume                     530.279
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            Tey_CMATEX_2006_828.cif
_cod_data_source_block           C3H12Li1N6Ni1O7.5
_cod_original_cell_volume        530.2794
_cod_original_formula_sum        'C3 H12 Li1 N6 Ni1 O7.5'
_cod_database_code               4002448
Synthesis, Structure, and Magnetic Properties of as Single Precursors to LiMO2 Battery Materials
Tey, S.L.; Reddy, M.V.; Rao, G.V.S.; Yi, J.; Vittal, J.J.; Chowdary, B.V.R.; Ding, J.; Chemistry of Materials (1,1989-) 18 (2006) 1587–1594; doi:

data_4002449
_publ_section_title
;
 Synthesis, Structure, and Magnetic Properties of as Single Precursors to
 LiMO2 Battery Materials
;
_journal_name_full               'Chemistry of Materials (1,1989-)'
_journal_page_first              1587
_journal_page_last               1594
_journal_volume                  18
_journal_year                    2006
_chemical_formula_sum            'C3 H12 Co Li N6 O7.5'
_chemical_name_systematic        '(Li (H2 O) Co (N2 H3 C O2)3) (H2 O)0.5'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.337
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.5324
_cell_length_b                   5.0019
_cell_length_c                   11.3136
_cell_volume                     538.985
_citation_journal_id_ASTM        CMATEX
_cod_data_source_file            Tey_CMATEX_2006_829.cif
_cod_data_source_block           C3H12Co1Li1N6O7.5
_cod_original_formula_sum        'C3 H12 Co1 Li1 N6 O7.5'
_cod_database_code               4002449
Solid state phase equilibria in the Er-Ni-P and Er-Ni-As systems at 800
Zelinska, M.; Zhak, O.; Pivan, J.Y.; Polianska. T.; Oryshchyn, S.; AnorganischeChemie, Organische 62 (2007) 1143–1152; doi:

data_1529069
_publ_section_title
;
 Solid state phase equilibria in the Er-Ni-P and Er-Ni-As systems at 800
;
_journal_name_full               ' AnorganischeChemie, Organische '
_journal_page_first              1143
_journal_page_last               1152
_journal_volume                  62
_journal_year                    2007
_chemical_formula_sum            'As2 Er Ni4'
_chemical_name_systematic        'Er Ni4 As2'
_space_group_IT_number           136
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.2162
_cell_length_b                   7.2162
_cell_length_c                   3.7573
_cell_volume                     195.656
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Zelinska_ZNBSEN_2007_1368.cif
_cod_data_source_block           As2Er1Ni4
_cod_original_cell_volume        195.6559
_cod_original_formula_sum        'As2 Er1 Ni4'
_cod_database_code               1529069
Solid state phase equilibria in the Er-Ni-P and Er-Ni-As systems at 800
Zelinska, M.; Zhak, O.; Oryshchyn, S.; Polianska. T.; Pivan, J.Y.; AnorganischeChemie, Organische 62 (2007) 1143–1152; doi:

data_1529070
_publ_section_title
;
 Solid state phase equilibria in the Er-Ni-P and Er-Ni-As systems at 800
;
_journal_name_full               ' AnorganischeChemie, Organische '
_journal_page_first              1143
_journal_page_last               1152
_journal_volume                  62
_journal_year                    2007
_chemical_formula_sum            'As7 Er2 Ni12'
_chemical_name_systematic        'Er2 Ni12 As7'
_space_group_IT_number           174
_symmetry_space_group_name_Hall  'P -6'
_symmetry_space_group_name_H-M   'P -6'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.3505
_cell_length_b                   9.3505
_cell_length_c                   3.7981
_cell_volume                     287.585
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Zelinska_ZNBSEN_2007_1369.cif
_cod_data_source_block           As7Er2Ni12
_cod_original_cell_volume        287.5853
_cod_database_code               1529070
Synthesis, crystal structures, metal - atom distribution and magnetic properties of Cr(5-x) Ti(x) Se8 (x = 2, 3, 4)
Wontcheu, J.; Kockelmann, W.; Huang Zhongle; Schnelle, W.; Bensch, W.; Solid State Sciences 9 (2007) 506–514; doi:

data_1529071
_publ_section_title
;
 Synthesis, crystal structures, metal - atom distribution and magnetic
 properties of Cr(5-x) Ti(x) Se8 (x = 2, 3, 4)
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              506
_journal_page_last               514
_journal_volume                  9
_journal_year                    2007
_chemical_formula_sum            'Cr3.072 Se8 Ti1.788'
_chemical_name_systematic        'Cr3.072 Ti1.788 Se8'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.796
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.3989
_cell_length_b                   7.1873
_cell_length_c                   11.7608
_cell_volume                     1047.958
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Wontcheu_SSSCFJ_2007_1395.cif
_cod_data_source_block           Cr3.072Se8Ti1.788
_cod_original_sg_symbol_Hall     '-C 2y '
_cod_database_code               1529071
Synthesis, crystal structures, metal - atom distribution and magnetic properties of Cr(5-x) Ti(x) Se8 (x = 2, 3, 4)
Wontcheu, J.; Kockelmann, W.; Schnelle, W.; Huang Zhongle; Bensch, W.; Solid State Sciences 9 (2007) 506–514; doi:

data_1529072
_publ_section_title
;
 Synthesis, crystal structures, metal - atom distribution and magnetic
 properties of Cr(5-x) Ti(x) Se8 (x = 2, 3, 4)
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              506
_journal_page_last               514
_journal_volume                  9
_journal_year                    2007
_chemical_formula_sum            'Cr1.973 Se8 Ti2.711'
_chemical_name_systematic        'Cr1.973 Ti2.711 Se8'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.66
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.3728
_cell_length_b                   7.167
_cell_length_c                   11.8301
_cell_volume                     1048.975
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Wontcheu_SSSCFJ_2007_1396.cif
_cod_data_source_block           Cr1.973Se8Ti2.711
_cod_original_sg_symbol_Hall     '-C 2y '
_cod_original_sg_symbol_H-M      'C 1 2/m 1 '
_cod_database_code               1529072
Synthesis, crystal structures, metal - atom distribution and magnetic properties of Cr(5-x) Ti(x) Se8 (x = 2, 3, 4)
Wontcheu, J.; Kockelmann, W.; Bensch, W.; Schnelle, W.; Huang Zhongle; Solid State Sciences 9 (2007) 506–514; doi:

data_1529073
_publ_section_title
;
 Synthesis, crystal structures, metal - atom distribution and magnetic
 properties of Cr(5-x) Ti(x) Se8 (x = 2, 3, 4)
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              506
_journal_page_last               514
_journal_volume                  9
_journal_year                    2007
_chemical_formula_sum            'Cr0.678 Se8 Ti4.03'
_chemical_name_systematic        'Cr0.678 Ti4.03 Se8'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.62
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.3688
_cell_length_b                   7.1688
_cell_length_c                   11.931
_cell_volume                     1057.853
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Wontcheu_SSSCFJ_2007_1397.cif
_cod_data_source_block           Cr0.678Se8Ti4.03
_cod_original_sg_symbol_Hall     '-C 2y '
_cod_original_sg_symbol_H-M      'C 1 2/m 1 '
_cod_database_code               1529073
Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in Li4SiO4-Li3PO4 Solid Electrolytes.
Deng, Yue; Eames, Christopher; Chotard, Jean-Noël; Lalère, Fabien; Seznec, Vincent; Emge, Steffen; Pecher, Oliver; Grey, Clare P.; Masquelier, Christian; Islam, M. Saiful; Journal of the American Chemical Society 137 (2015) 9136–9145; doi:10.1021/jacs.5b04444

data_4124125
_publ_section_title
;
 Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in
 Li4SiO4-Li3PO4 Solid Electrolytes.
;
_journal_issue                   28
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9136
_journal_page_last               9145
_journal_paper_doi               10.1021/jacs.5b04444
_journal_volume                  137
_journal_year                    2015
_chemical_formula_structural     Li6.5Si0.5P1.5O8
_chemical_formula_sum            'Li6.5 O8 P1.5 Si0.5'
_chemical_formula_weight         233.57
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_formula_units_Z            2
_cell_length_a                   10.52587(9)
_cell_length_b                   6.11525(6)
_cell_length_c                   4.97031(5)
_cell_measurement_temperature    300
_cell_volume                     319.931(5)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      300
_diffrn_radiation_type           'Constant Wavelength Neutron Diffraction'
_diffrn_radiation_wavelength     1.59464
_diffrn_source                   'nuclear reactor'
_pd_instr_location
;
;
_pd_meas_2theta_range_inc        0.050018
_pd_meas_2theta_range_max        159.95000
_pd_meas_2theta_range_min        0.00000
_pd_meas_number_of_points        3200
_pd_proc_2theta_range_inc        0.050018
_pd_proc_2theta_range_max        159.7681
_pd_proc_2theta_range_min        -0.1819
_pd_proc_ls_pref_orient_corr
;
;
_pd_proc_ls_prof_R_factor        2.7512
_pd_proc_ls_prof_wR_expected     2.0894
_pd_proc_ls_prof_wR_factor       3.5448
_pd_proc_wavelength              1.594644
_pd_spec_mounting
;
;
_refine_ls_goodness_of_fit_all   2.8783
_refine_ls_number_parameters     72
_refine_ls_number_reflns         353
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            3.7004
_cod_data_source_file            ja5b04444_si_002.cif
_cod_data_source_block           Li3.25Si0.25P0.75O4
_cod_depositor_comments
'Adding full bibliography for 4124125--4124128.cif.'
_cod_original_cell_volume        319.930(5)
_cod_original_formula_sum        Li6.5O8P1.5Si0.5
_cod_database_code               4124125
_publcif_datablock.id            {a5284229-5a5c-41fa-b2df-c2fc0b64f231}
_pd_proc_ls_prof_cr_factor       11.8479
_pd_proc_ls_prof_cwr_factor      10.7056
_pd_proc_ls_prof_cwr_expected    6.3101
_pd_proc_ls_prof_chi2            2.8783
_pd_proc_ls_prof_echi2           2.9091
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in Li4SiO4-Li3PO4 Solid Electrolytes.
Deng, Yue; Eames, Christopher; Chotard, Jean-Noël; Lalère, Fabien; Seznec, Vincent; Emge, Steffen; Pecher, Oliver; Grey, Clare P.; Masquelier, Christian; Islam, M. Saiful; Journal of the American Chemical Society 137 (2015) 9136–9145; doi:10.1021/jacs.5b04444

data_4124126
_publ_section_title
;
 Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in
 Li4SiO4-Li3PO4 Solid Electrolytes.
;
_journal_issue                   28
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9136
_journal_page_last               9145
_journal_paper_doi               10.1021/jacs.5b04444
_journal_volume                  137
_journal_year                    2015
_chemical_formula_structural     Li7Si1P1O8
_chemical_formula_sum            'Li7 O8 P Si'
_chemical_formula_weight         235.60
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_formula_units_Z            2
_cell_length_a                   10.58917(10)
_cell_length_b                   6.11520(6)
_cell_length_c                   5.00565(4)
_cell_measurement_temperature    300
_cell_volume                     324.140(5)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      300
_diffrn_radiation_type           'Constant Wavelength Neutron Diffraction'
_diffrn_radiation_wavelength     1.59464
_diffrn_source                   'nuclear reactor'
_pd_instr_location
;
;
_pd_meas_2theta_range_inc        0.050018
_pd_meas_2theta_range_max        159.95000
_pd_meas_2theta_range_min        0.00000
_pd_meas_number_of_points        3200
_pd_proc_2theta_range_inc        0.050018
_pd_proc_2theta_range_max        159.7658
_pd_proc_2theta_range_min        -0.1842
_pd_proc_ls_pref_orient_corr
;
;
_pd_proc_ls_prof_R_factor        2.9333
_pd_proc_ls_prof_wR_expected     1.9912
_pd_proc_ls_prof_wR_factor       3.8832
_pd_proc_wavelength              1.594644
_pd_spec_mounting
;
;
_refine_ls_goodness_of_fit_all   3.8032
_refine_ls_number_parameters     70
_refine_ls_number_reflns         362
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            4.9228
_cod_data_source_file            ja5b04444_si_002.cif
_cod_data_source_block           Li3.50Si0.50P0.50O4
_cod_depositor_comments
'Adding full bibliography for 4124125--4124128.cif.'
_cod_original_formula_sum        Li7O8P1Si1
_cod_database_code               4124126
_publcif_datablock.id            {be56cd62-9fa6-405c-8561-2494a58725c3}
_pd_proc_ls_prof_cr_factor       15.0794
_pd_proc_ls_prof_cwr_factor      12.8766
_pd_proc_ls_prof_cwr_expected    6.6027
_pd_proc_ls_prof_chi2            3.8032
_pd_proc_ls_prof_echi2           3.8505
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in Li4SiO4-Li3PO4 Solid Electrolytes.
Deng, Yue; Eames, Christopher; Chotard, Jean-Noël; Lalère, Fabien; Seznec, Vincent; Emge, Steffen; Pecher, Oliver; Grey, Clare P.; Masquelier, Christian; Islam, M. Saiful; Journal of the American Chemical Society 137 (2015) 9136–9145; doi:10.1021/jacs.5b04444

data_4124127
_publ_section_title
;
 Structural and Mechanistic Insights into Fast Lithium-Ion Conduction in
 Li4SiO4-Li3PO4 Solid Electrolytes.
;
_journal_issue                   28
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              9136
_journal_page_last               9145
_journal_paper_doi               10.1021/jacs.5b04444
_journal_volume                  137
_journal_year                    2015
_chemical_formula_structural     Li7.50Si1.50P0.50O8
_chemical_formula_sum            'Li7.5 O8 P0.5 Si1.5'
_chemical_formula_weight         238
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.3692(8)
_cell_angle_gamma                90.00000
_cell_formula_units_Z            1
_cell_length_a                   5.10536(11)
_cell_length_b                   6.11225(12)
_cell_length_c                   5.29671(11)
_cell_measurement_temperature    300
_cell_volume                     165.282(6)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      300
_diffrn_radiation_type           'Constant Wavelength Neutron Diffraction'
_diffrn_radiation_wavelength     1.49400
_diffrn_source                   'nuclear reactor'
_pd_instr_location
;
;
_pd_meas_2theta_range_inc        0.050000
_pd_meas_2theta_range_max        164.70000
_pd_meas_2theta_range_min        3.75000
_pd_meas_number_of_points        3220
_pd_proc_2theta_range_inc        0.050000
_pd_proc_2theta_range_max        164.8293
_pd_proc_2theta_range_min        3.8793
_pd_proc_ls_pref_orient_corr
;
;
_pd_proc_ls_prof_R_factor        3.3129
_pd_proc_ls_prof_wR_expected     3.4220
_pd_proc_ls_prof_wR_factor       4.3091
_pd_proc_wavelength              1.494000
_pd_spec_mounting
;
;
_refine_ls_goodness_of_fit_all   1.5857
_refine_ls_number_parameters     78
_refine_ls_number_reflns         449
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            2.4358
_cod_data_source_file            ja5b04444_si_002.cif
_cod_data_source_block           Li15Si3PO16
_cod_depositor_comments
'Adding full bibliography for 4124125--4124128.cif.'
_cod_original_cell_volume        165.281(6)
_cod_original_sg_symbol_H-M      'P 21/m'
_cod_original_formula_sum        Li7.50O8P0.50Si1.50
_cod_database_code               4124127
_publcif_datablock.id            {cc97d60d-c88d-4ce6-a989-7472f2f8cd81}
_pd_proc_ls_prof_cr_factor       7.9979
_pd_proc_ls_prof_cwr_factor      8.9474
_pd_proc_ls_prof_cwr_expected    7.1055
_pd_proc_ls_prof_chi2            1.5857
_pd_proc_ls_prof_echi2           1.5981
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
Global instability index optimisation for the localization of mobile protons
Adams, S.; Moretzki, O.; Canadell, E.; Solid State Ionics 168 (2004) 281–290; doi:

data_1529095
_publ_section_title
;
 Global instability index optimisation for the localization of mobile
 protons
;
_journal_name_full               'Solid State Ionics'
_journal_page_first              281
_journal_page_last               290
_journal_volume                  168
_journal_year                    2004
_chemical_formula_sum            'H0.95 Mo O3'
_chemical_name_systematic        'H0.95 (Mo O3)'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-I 2y'
_symmetry_space_group_name_H-M   'I 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 93.727
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   14.5263
_cell_length_b                   3.7944
_cell_length_c                   7.7219
_cell_volume                     424.720
_citation_journal_id_ASTM        SSIOD3
_cod_data_source_file            Adams_SSIOD3_2004_11.cif
_cod_data_source_block           H0.95Mo1O3
_cod_original_cell_volume        424.7201
_cod_original_sg_symbol_Hall     '-C 2y (x,y,-x+z)'
_cod_original_formula_sum        'H0.95 Mo1 O3'
_cod_database_code               1529095